Abstract
Significant progress has been made in superconducting quantum circuits. However new quantum devices that have longer decoherence times at higher temperatures are urgently required for quantum technologies. Superconducting nanowires with quantum phase slips are promising candidates for use in novel quantum devices. Here, we demonstrate YBa_{2}Cu_{3}O_{7x} nanowires with phaseslip dynamics and study their switchingcurrent statistics at temperatures below 20 K. We apply theoretical models developed for Josephson junctions and show that our results provide strong evidence for energylevel quantization in the nanowires. The crossover temperature to the quantum regime of 12–13 K and the lifetime in the excited state exceeding 20 ms at 5.4 K are superior to those in conventional Josephson junctions. We also show how the absorption of a single photon changes the phaseslip and quantum state of a nanowire, which is important for the development of singlephoton detectors with high operating temperature and superior temporal resolution.
Introduction
Superconducting quantum circuits are based on electrical inductorcapacitor (LC) oscillators, in which the Josephson effect contributes the nonlinearity that is required for selective access to quantum levels^{1}. Historically, tunnel Josephson junctions (JJs) have played a major role in studies of macroscopic quantum phenomena and, nowadays, most superconducting quantum circuits are based on them. However, the Josephson effect also occurs in structures with a nontunneling conductivity, which together with tunnel JJs form a class of superconducting weak links^{2}. Nanowires with quantum phase slips caused by fluctuations of the order parameter are particularly interesting superconducting weak links with direct conductivity, as they can be used in superconducting quantum circuits^{3,4,5,6}. The potential of these nanowires lies in their longlived excited states, which result from their low sensitivity to charge noise and critical current noise^{3}. The electrodynamics of superconducting nanowires with strong fluctuations of the order parameter are not well understood, but are likely to be governed by principles similar to those for single JJs. Notably, it is possible to describe both systems by the resistively and capacitively shunted junction (RCSJ) model^{7,8,9}, when applying minor modifications that account for the differences between phaseslip nanowires (PSNs) and JJs (see Supplementary Note 1). Here, we use the term PSN to refer to a superconducting nanowire that has a finite critical current and the resistive state occurring due to phase slippage.
A tunnel JJ exhibits two macroscopic quantum phenomena that are important for quantum circuits: macroscopic quantum tunneling (MQT) and energylevel quantization (ELQ) that were experimentally observed for JJs from lowtemperature (lowT_{c}) and hightemperature (highT_{c}) cuprate superconductors^{10,11,12,13,14,15}. MQT has been demonstrated for PSNs fabricated from different lowT_{c} superconductors^{16,17,18}. However, there is a significant difference between a JJ and a lowT_{c} PSN, because the physical mechanisms that determine the frequency of plasma oscillations have a very different nature. The zerobias plasma frequency of a JJ ω_{p0} = (2eI_{c}/Cħ)^{1/2} (referred to as a Josephson plasma frequency) is given by the resonant frequency of an L_{J}C circuit consisting of a Josephson inductance L_{J} = ħ/2eI_{c}cosφ and a junction capacitance C^{19}. Here, I_{c} is critical current, e is the electron charge, ħ = h/2π is reduced Planck’s constant, and φ is phase difference across a JJ. When compared with tunnel JJs, the nanowires typically have very small intrinsic capacitances. In a lowT_{c} nanowire, the energy of Josephson plasma oscillations is much higher than the superconducting energy gap 2Δ, which makes such oscillations impossible, as shown in Fig. 1a. In a pioneering study^{16}, Giordano proposed that the plasma frequency of lowT_{c} PSNs is limited by another physical mechanism and scales with Δ. This was experimentally confirmed by measurements of the crossover temperature between MQT and thermal activation (TA) escape mechanisms for different lowT_{c} PSNs^{17,18}. As a result of the very high plasma frequency, it is therefore unlikely that more than one energy level exists in a lowT_{c} PSN.
In contrast, in highT_{c} superconductors the superconducting energy gap is much larger and Josephson plasma oscillations are allowed, as shown in Fig. 1a. In addition to having a large superconducting energy gap of Δ = 25–30 meV^{20}, YBa_{2}Cu_{3}O_{7−x} (YBCO) nanowires demonstrate a singlevalued sinelike currentphase relation, even at temperatures close to zero^{21}.
Here, we show that YBCO nanowires are promising candidates for realizing superconducting quantum circuits. Our measurements of switchingcurrent statistics for ultrathin YBCO nanowires with phaseslip dynamics provide clear evidence of ELQ in the nanowires.
Results
Energylevel quantization
We performed electrical transport measurements on 2μmlong 8.2nmthick YBCO nanowires with nominal widths <300 nm on a (100) SrTiO_{3} (STO) substrate. Figure 1b shows a scanning electron micrograph of a representative nanowire patterned using focused ion beam (FIB) milling across a 10μmwide microbridge. All of the nanowires showed current–voltage (IV) curves that were characteristic of phase slippage, as described in previous work^{22}. Based on the linear dependence of the critical current and normalstate resistance on nominal nanowire width and thickness, we determined the effective nanowire width and thickness that we use below rather than the nominal ones. Significantly, the switchingcurrent statistics of nanowires with effective widths of <100 nm cannot be explained using models developed for lowT_{c} nanowires. For a nanowire with an effective thickness and width of 4.3 and 55 nm, respectively, we observe current–voltage characteristics that show direct voltage switching from the superconducting to the resistive state and large current hysteresis over an extended temperature range of up to 18–20 K, as shown in Fig. 1c. Onedimensional phaseslip centers described by the Skocpol–Beasley–Tinkham model^{23} can appear in superconducting nanowires with width W ≤ 4.4ξ^{2,24}, where ξ denotes the coherence length. In wider nanowires, a phase slippage occurs either by the twodimensional analog of a phaseslip center (i.e., the order parameter is suppressed across the entire nanowire) or a socalled vortex street (i.e., running phaseslip centers, which are also referred to as kinematic vortices)^{25,26}. For our nanowires W > 40ξ and we hence consider the vortex street mechanism as energetically favorable. Note that we will refer to the phaseslip process in our YBCO nanowires using the wellestablished term “phaseslip line”, bearing in mind that the phase slippage occurs due to the motion of kinematic vortices. To observe phase slippage in wide nanowires, as is the case here, it is necessary to realize nanowires with smooth edges and efficient heat removal^{26,27}. We calculate the Ginzburg–Landau depairing current density as J_{GL} = Φ_{0}/3^{3/2}πμ_{0}λ^{2}ξ ≈ 390 MA cm^{−2}, where Φ_{0} is the magnetic flux quantum, μ_{0} is the vacuum permeability, λ = 140 nm^{28}, and ξ = 1.3 nm^{29} are the magnetic field penetration depth and the coherence length at zero temperature, and find that order parameter fluctuations significantly reduce the critical current density to ~20% of J_{GL} for our YBCO nanowires.
To assess the possibility of ELQ in a 55nmwide nanowire, we use the extended RCSJ model (Supplementary Note 1). We calculate the zerobias plasma frequency, ω_{p0}/2π = (2eI_{c}/ħC_{nw})^{1/2} ≈ 1.6 THz, for such nanowire with capacitance C_{nw} = 4.8 fF (Methods section), assuming that the switching current is close to the critical current I_{c}. The energy of corresponding Josephson plasma oscillations ω_{p0}ħ = 6.6 meV is significantly lower than 2Δ_{0} = 50–60 meV. Hence, several quantized energy levels can exist in the nanowire. Assuming that the losses are mainly due to thermally equilibrium quasiparticles, we estimate the quality factor of the nanowire in the superconducting state as Q_{s} = ω_{p0}R_{qp}C_{nw} = (2eI_{c}C_{nw}/ħ)^{1/2}R_{n}e^{Δ/kT} ≈ 10^{32}–10^{10} in the 4–15 K temperature range, where R_{qp} = R_{n}e^{Δ/kT} is the quasiparticle resistance, R_{n} = 4200 Ω is the normalstate resistance of the nanowire, k is the Boltzmann constant, and Δ = 25 meV. The exponential temperature dependence of the quasiparticle number in superconductors is only observable until a certain temperature due to the presence of twolevel fluctuators and coupling to the environment. Note that in the case of YBCO, the exponential dependence would already provide for an excited state lifetime of 10 years at the temperature of 6.5 K that is sufficient for practical applications.
The registration of the escape from a potential well either by TA or MQT significantly depends on the damping in the resistive state. Within the framework of the mechanical analog of the RCSJ model, which considers the motion of a particle in a washboard potential, the system stops in the nearest local minimum after the escape event if the damping is high. The resulting short voltage pulse is very difficult to detect. If the damping is low, the particle continues to move along a tilted washboard potential after a singleescape event, even when the washboard potential has local minima. The phase difference is free running and some finite voltage appears across the JJ, which is straightforward to detect with a voltmeter. The crossover between the low and highdamping regimes take place at a quality factor of Q = 0.8382 (ref. ^{30}). Here, we use similar criteria to evaluate the behavior of a phaseslip nanowire after an escape event. We calculate the quality factor of the nanowire in the resistive state as Q_{n} = (2e/h)(2Λ_{Q}/L)V_{s}R_{ps}C_{nw} ≈ 1 (Supplementary Note 1), where R_{ps} = 120 Ω is the phaseslip line resistance, V_{s} = 2.7 mV is the voltage switching amplitude, and Λ_{Q} = 200 nm is the charge imbalance distance^{22}. We conclude that the nanowire will switch into the resistive state after a singleescape event because Q_{n} > 0.8382 and the tunneling from different energy levels can be detected by measuring the switching current. Furthermore, we expect a crossover between TA and MQT escape mechanisms at a temperature of T_{cr} ≈ ω_{p0}ħ/2πk = 12.4 K^{19}. Based on these calculations, we conclude that the energy levels in our YBCO PSNs must be quantized at low temperatures and can be revealed using switchingcurrent measurements.
Nanowire under equilibrium conditions
We measured switchingcurrent statistics for a 55nmwide 4.3nmthick YBCO nanowire, both under equilibrium conditions and under illumination with 77 K black body radiation (BBR) as well as visible light, inducing nonequilibrium states of the wire. In order to reach thermal equilibrium of the nanowire with external radiation, we kept the radiation shield surrounding the nanowire and the nanowire itself at the same temperature. We recorded 1500 IV curves with a current sweep rate of dI/dt = 0.55 mA s^{−1} for each of eight distinct temperatures in the 4.2–18 K temperature range, determined the switchingcurrent values and extracted the switchingcurrent distributions (SCDs), which are shown in Fig. 2a. The measured SCDs represent the probability of the decay of the zerovoltage state when the bias current is ramped up. The decay of the zerovoltage state occurs by the TA or MQT with rate that exponentially depends on the bias current^{31}. At the highest temperature of 18 K, the SCD shows a single peak at a switching current of 156.12 μA. As the temperature is decreased to 16–14 K, the SCD peak shifts to higher switching currents, broadens, and develops an asymmetry with a fine structure of closely spaced peaks with spacings of 74 ± 20 nA and 116 ± 31 nA, respectively (enlarged SCDs are shown in Supplementary Fig. 1). Below 14 K, the SCDs show new peaks on either side of the main peak. This threepeaked structure is most pronounced close to 10 K and gradually disappears at 6–4.2 K.
Within the framework of the RCSJ model, the switching and retrapping processes are affected by external noise in a similar way. We measure retrappingcurrent distributions (RCDs) simultaneously with the SCD and find only a single peak with standard deviation σ_{r} = 62.8 ± 3.6 nA for all temperatures, indicating that the SCD transformation is caused by intrinsic nanowire dynamics rather than by external noise (RCDs are shown in Supplementary Fig. 2).
The only model that predicts the broadening and oscillations of the SCD at temperatures slightly above the TA–MQT crossover temperature T_{cr} = 12.4 K was given by Silvestrini et al.^{32,33}, who considered the dependence of SCDs on the bias current ramp rate. The model predicts that the decay from lower energy levels becomes accessible at temperatures slightly above the crossover temperature, if the bias current ramp rate is high enough, i.e., nonadiabatic. The nonadiabatic transition between the TA and MQT regimes is shown schematically in Fig. 2b–g. At temperatures well below T_{cr}, only the lowest (ground) energy level is populated (Fig. 2b). Escape is dominated by MQT from the groundstate energy level and the corresponding SCD is single peaked and narrow (Fig. 2e). When the temperature is close to T_{cr}, higher energy levels become populated as a result of thermal fluctuations (Fig. 2c), according to a Boltzmann distribution. If the current sweep rate is high, so that the upper energy level cannot be refilled by thermal fluctuations, then escape from the lower energy levels becomes possible and the nanowire can switch into a resistive state over a wider current range. The corresponding SCD (Fig. 2f) is broad and has a fine structure of closely spaced peaks caused by escape from different energy levels. At temperatures well above the crossover temperature, the energy levels are broadened and their superposition forms a continuous energy band, as shown in Fig. 2d. The nanowire switches into the resistive state via TA from the upper edge of this energy band, resulting in a singlepeaked and narrow SCD (Fig. 2g). Nonadiabatic broadening of the SCD can be observed experimentally, when the current sweep rate dI/dt > I_{c}/200R_{qp}C, where R_{qp} is the quasiparticle resistance^{32}. By using this expression, we obtain an orderofmagnitude estimate of the quasiparticle resistance, R_{qp} ≈ 3 × 10^{11} Ω and find the quality factor in the superconducting state Q_{s} = ω_{p0}R_{qp}C ≈ 1.5 × 10^{10} as well as the lifetime in the excited state τ = Q_{s}/ω_{p0} ≈ 1.5 ms at T = 14–16 K. The quality factor in the superconducting state is in good agreement with our estimates made within the extended RCSJ model. We attribute the presence of smaller peaks on both sides of the main peak in the SCD at T < T_{cr} to interaction of the nanowire plasma oscillations with an external resonant system, i.e., with geometric resonances of the 10μmlong microbridge or the bowtie antenna of our device (Methods section), with resonant frequencies of 1.2 THz and 40 GHz, respectively.
In order to probe the energylevel structure in the PSN under equilibrium conditions, we applied external noise to the nanowire via the cables connecting the Dewar insert to the measurement equipment. We found that external noise has a significant effect on the SCDs, as shown in Fig. 3a for three different temperatures at a current sweep rate dI/dt = 2.75 mA s^{−1}. At 4.2 K, the SCD consists of four nearly equally spaced peaks, which are marked I_{s1} – I_{s4} in Fig. 3a. At 5.9 K, the spacing between the peaks decreases slightly. At 8 K, only two peaks remain in the SCD. The noiseaffected RCD shows only a single peak with σ_{r} = 51 ± 3 nA (Supplementary Fig. 3), indicating that the applied lowfrequency noise does not cause the multiple peak structure in the SCD, but acts as a trigger for another physical mechanism, which is discussed below.
The nearly evenly paced peaks I_{s1} – I_{s4} in Fig. 3a are signatures of tunneling from different energy levels, as shown in Fig. 3b. If the damping is moderate, i.e., if the quality factor is close to unity, then a particle that escaped from the potential well due to external noise activation (magenta arrow) can be trapped in the upper energy level of the lower potential well. This retrapping process in a PSN is similar to that of thermal or quantum phase diffusion in underdamped tunnel JJs^{34,35}. When a particle is trapped in the upper energy level, it can decay to lower energy levels in the same well (blue arrows) or escape from the potential well by tunneling (red arrows), resulting in the presence of multiple peaks in the SCD. Within the framework of this model, the I_{s1} – I_{s4} values are given by a system of equations ΔU(I_{si}) = ΔU_{tun} + E_{n}(I_{si}) (1), where i is an integer, and ΔU(I_{si}) and E_{n}(I_{si}) are the energy barrier height and the energy of the populated energy level corresponding to escape at current I_{si}, respectively. Here, we assume that the particle tunnels through the barrier when the barrier height for the populated energy level is decreased to ΔU_{tun}. We approximate the nanowire by a harmonic quantum oscillator with energy levels E_{n}(I_{si}) = ω_{p}(I_{si})ħ(n + 1/2), where ω_{p} is the currentdependent plasma frequency. We also use the approximate expressions for barrier height ΔU(I) = (hI_{c}/2πe)[(1 − (I/I_{c})^{2})^{1/2} − (I/I_{c})arccos(I/I_{c})]^{36} and plasma frequency ω_{p}(I) = ω_{p0}[1 − (I/I_{c})^{2}]^{1/4} (ref. ^{19}). By solving the system of equations (1), we obtain ω_{p0}/2π = 744 GHz. We analyze the stability of the solution under small perturbations of the initial parameters and find that the realvalued solution disappears, when the I_{si} values are varied by >100 nA from their initial values. Hence, we conclude that the observed peaks I_{s1} – I_{s4} can indeed be assigned to energy levels in a tilted washboard potential. We note that the calculated zerobias plasma frequency is only approximately half of our previous estimate based on the nanowire capacitance and the crossover temperature. Using the numerically simulated eigenvalues E_{n}/ω_{p}ħ of the JJ in a cubic approximation of the washboard potential, which take values of 0.5, 1.45, and 2.37 for n = 0, 1 and 2 (ref. ^{36}), we obtain the ω_{p0}/2π value as 1.5 THz, which is close to our theoretical estimate. The reduced number of peaks in the SCD at 8 K can be attributed to a decrease in energy level lifetime with increasing temperature when transitions to the lower energy level become more probable than tunneling through the barrier.
Nanowire under illumination with BBR
In order to probe the energylevel structure of the nanowire using external radiation, we illuminated the device with 77 K BBR, which has a broad continuous spectrum peaked at a frequency of 8 THz and can populate energy levels up to 2Δ, resulting in a nonequilibrium state of the nanowire. We studied the resulting nonequilibrium nanowire state in the 5.4–20.1 K temperature range using three current sweep rates of 0.055, 0.55, and 2.75 mA s^{−1}. The resulting SCDs (orange bars) are shown in Fig. 4a–d. Well above the crossover temperature, the SCD does not show any sign of quantized energy levels (Fig. 4a), similar to experiments with the nanowire under equilibrium conditions.
When the temperature is close to the crossover temperature (Fig. 4b), the SCD has a single peak at the lowest current sweep rate dI/dt = 0.055 mA s^{−1}, which broadens toward higher currents with increasing current sweep rate, eventually transforming into a distribution with two peaks at dI/dt = 2.75 mA s^{−1}. This transformation of the SCD with current sweep rate reflects a transition from adiabatic to nonadiabatic measurements, as lower energy levels become accessible. Below the crossover temperature, at 10.9 K, we observe a strong dependence of the spectral weight of the peak I_{s2} on the current sweep rate, as shown in Fig. 4c. At even lower temperature (5.4 K in Fig. 4d), the spectral weight dependence of the I_{s2} peak with current sweep rate is less pronounced and the I_{s1} peak is hardly observable.
We interpret the difference in spectral weight between the peaks at I_{s1} and I_{s2} in terms of a population inversion resulting from the decay of higherlying energy levels, similar to observations in superconducting quantum circuits based on tunnel JJs^{37,38}. We identify the I_{s1} and I_{s2} peaks in Fig. 4c, d with the ground and first exited energy levels, respectively. The effects of temperature and current sweep rate on the spectral weights of the I_{s1} and I_{s2} peaks can then be assessed using the tilted washboard potential model, as shown in Fig. 4e. Tunneling from the ground, first and second excited energy levels occurs at currents I_{1}, I_{2}, and I_{3}, respectively. Population inversion in the steady state is possible for currents I < I_{3} when three or more energy levels exist in the potential well. At I_{3} ≤ I < I_{2}, the number of the energy levels is reduced to two and the nanowire state evolves toward a steady state, with similar population probabilities for the ground and first excited states by spontaneous and stimulated transitions during the time t_{32} = [I_{3} – I_{2}]/(dI/dt) ≈ [I_{2} – I_{1}]/(dI/dt). The nanowire quantum state can be read out at I = I_{2} or I_{1}. As the energylevel occupation probability depends strongly on temperature and current bias sweep rate, the spectral weight of the SCD peak at I = I_{2} decreases with increasing temperature or with decreasing current sweep rate.
We calculate the lifetime in the exited state by associating the spectral weight of the I_{s2} peak with the occupation probability of the first excited energy level P_{2}(t). A fit of the expression A + B × exp(−t/τ_{2}) to the experimental data (Supplementary Fig. 4) yields reasonable fitting parameters of A = 0.55 and B = 0.39, and an excited state lifetime of τ_{2} = 8.3 ms. Assuming that the lifetime τ_{2} at 10.9 K is limited by quasiparticle losses and considering the nanowire as a lumped element with quasiparticle resistance R_{qp} = R_{n} × e^{Δ/kT}, where R_{n} ≈ 4200 Ω is the normalstate nanowire resistance, we obtain a reasonable estimate of the superconducting energy gap in YBCO Δ(10.9 K) = kTln(τ_{2}/2πCR_{n}) ≈ 17 meV. The lifetime in the excited state τ_{2} at 5.4 K is, however, much longer than t_{32} ≈ 20 ms, because we only observe a minimal dependence of the population probability P_{2}(t) of the first exited level on the current sweep rate down to dI/dt = 55 μA s^{−1}. The RCDs show only a single peak for all temperatures and current sweep rates, as illustrated by the blue bars in Fig. 4a–d. We find the standard deviations of the retrapping current of 88.1 ± 5.7, 67.9 ± 4.4, and 56.8 ± 5.0 nA at dI/dt of 0.055, 0.55, and 2.75 mA s^{−1}, respectively and are able to reproduce similar σ_{r} values with two different experimental setups, confirming that switching into the resistive state originates from internal nanowire dynamics and not external noise.
Singlephoton control of YBCO PSNs
Additional illumination of the nanowire using optical radiation with an lightemitting diode (LED) led to seemingly counterintuitive results: the number of switching events with higher switching current was observed to increase with increasing LED irradiance. Representative SCDs measured at different irradiances of a blue LED with 460 nm wavelength for a current sweep rate of dI/dt = 0.55 mA s^{−1} are shown in Fig. 5a. When the LED is turned off, the nanowire is still subjected to 77 K BBR and switches into the resistive state in current range II (Fig. 5a), which corresponds to tunneling from the first exited state of the nanowire. At an LED irradiance of I_{LED} = 0.7 W m^{−2}, switching events occur not only in region II but also in region I of the current range in Fig. 5a, which corresponds to tunneling from the ground energy state. As the LED irradiance rises, the number of switching events in current region I increases and some switching events start to appear in the gap between current regions I and II, forming a peak at I = 186.5 μA when I_{LED} = 8.3 W m^{−2}.
The interaction of optical photons with a superconducting nanowire has been studied widely because of its practical importance for the development of superconducting nanowire singlephoton detectors^{39,40,41,42}. Here, we use a refined hotspot model to analyze singlephoton effects in YBCO nanowires^{42}. An optical photon whose energy is much higher than the superconducting energy gap disrupts tens of Cooper pairs, resulting in the appearance of nonequilibrium quasiparticles. The absorbed photon induces a normalstate domain (hotspot) across the nanowire when the number of nonequilibrium quasiparticles reaches N_{q} = n_{s}Wd(πDτ_{th})^{1/2}(1 − I/I_{c}), where n_{s} is the local density of paired electrons, d is the nanowire thickness, D is the quasiparticle diffusion coefficient, and τ_{th} is the quasiparticle thermalization time^{42}. We consider the quasiparticle motion during the thermalization process to be diffusive because the electron–electron scattering time τ_{e−e} = 0.1 ps^{43,44} in YBCO is much shorter than the thermalization time τ_{th} = 0.56 ps^{43,45}. If the entire photon energy E_{ph} is transferred to the quasiparticles, their actual number is given by N_{q} = E_{ph}/Δ. The boundary for hotspot appearance can then be calculated as I_{HS} = I_{c} – [j_{c}E_{ph}/n_{s}Δ(πDτ_{th})^{1/2}], where j_{c} is the critical current density. Photon absorption below and above I_{HS} has qualitatively different consequences. For I < I_{HS}, the photon creates nonequilibrium quasiparticles, but the normalstate domain across the nanowire does not appear. For I > I_{HS}, photon absorption results in a hotspot across the nanowire, which leads to local collapse of the order parameter. The PSN evolves from this transient state toward a state with a phaseslip process, corresponding to switching of the nanowire from the superconducting to the resistive state, as described in ref. ^{46}.
For photons of wavelength 460 nm, we calculate I_{c} − I_{HS} = j_{c}E_{ph}/n_{s}Δ(πDτ_{th})^{1/2} = 1.1–1.3 μA using n_{s} = 1.1·10^{27} m^{−3} (ref. ^{47}), Δ = 25–30 meV, D = 20 cm^{2} s^{−1} (ref. ^{44}), τ_{th} = 0.56 ps^{43,45}, E_{ph} = 2.7 eV, and the experimentally measured j_{c} = 78.6 MA cm^{−2}. In Fig. 5a, we highlight this current region III in red, in which the nanowire can switch to the resistive state only by the 460 nm wavelength photons. We assume that the critical current in the refined hotspot model corresponds to the switching current of the nanowire in the ground energy state.
Figure 5b illustrates schematically the interaction of optical photons with a PSN that has quantized energy levels and is prepared in the excited state. When the LED is turned off, the nanowire switches to a resistive state at current I_{2} due to tunneling from the first excited energy state. At a low LED irradiance (I_{LED} = 0.7 W m^{−2} in Fig. 5a), the nanowire can absorb the photon before reaching current I_{2}. Since photon absorption takes place at I < I_{HS}, it creates a number of nonequilibrium quasiparticles, resulting in an increase in nanowire losses, which is shown in Fig. 5b by a broadening of the energy levels and, hence, faster decay from the excited to the ground energy state. Switching into the resistive state then occurs at the higher current I_{1} by tunneling from the ground energy level. Therefore, the nanowire quantum state can be changed by singlephoton absorption.
When the radiation irradiance is increased (corresponding to high LED irradiance in Fig. 5b, and I_{LED} = 1.4–5.5 W m^{−2} in Fig. 5a), the nanowire can absorb a second photon at bias currents of I > I_{HS}, where hotspot conditions are met. As a result of the local collapse of the order parameter, the oscillating phaseslip process appears and the nanowire switches into the resistive state. Since the absorbed photon changes the number of phaseslip processes in the nanowire, i.e., the phaseslip state of the nanowire, we refer to this process as the phaseslip mechanism for photon detection.
At very high radiation irradiances, switching of the nanowire occurs predominantly at the boundary of the hotspot region, forming a peak in the SCD at I = I_{HS}. We observe this very high irradiance regime at I_{LED} = 8.3 W m^{−2} in Fig. 5a, where a peak at the edge of region III is visible. We treat the observed interaction of the optical photons with the YBCO nanowire as a singlephoton process because the position of the photoninduced SCD peak corresponds to the singlephoton energy and the radiation power is much lower than that required for the twophoton process. Comparing the LED irradiance to the W = 55 nm wide and L = 2μmlong nanowire, we estimate that no more than N = (ηLWI_{LED})/E_{ph} ≈ 53,000–630,000 photons s^{−1} are absorbed by the nanowire, where I_{LED} = 0.7–8.3 W m^{−2} is the LED irradiance, and η ≈ 0.3 is the theoretical estimate for the absorption coefficient of a metal film, which we calculate from the YBCO film sheet resistance R_{s} = 115 Ω at temperatures just above T_{c}^{48}. The average photon absorption rate hence is in the range of one photon per 1.6–19 μs. This time interval is approximately six orders of magnitude longer than the quasiparticle recombination time, τ_{r} = 3–10 ps, in optimally doped YBCO thin films on STO substrates or singlecrystal samples^{49,50}. The perturbation caused by the absorption of a photon will thus decay long before a subsequent photon will be absorbed in the nanowire. Based on the above, we consider our nanowire to be in the singlephoton regime where multiphoton processes occur with extremely low probability and can be neglected.
In this work, we have implicitly considered a nanowire made from YBCO, which has d_{x2−y2}wave symmetry of the order parameter as a fully gapped superconductor. We find that a small (N_{q} ≤ 100) number of nonequilibrium quasiparticles generated by an optical photon is significantly larger than the number of equilibrium quasiparticles in the nanowire, resulting in fast decay from the excited to the ground state. This behavior is expected for a fully gapped superconductor with an exponentially small number of equilibrium quasiparticles at a temperature well below the critical temperature. Deviations from d_{x2−y2}wave symmetry in our YBCO nanowires can arise from size or doping effects, which have recently been observed in different cuprate superconductors^{51,52}.
Discussion
In summary, we have fabricated sub100nmwide YBCO nanowires with phaseslip dynamics and measured their switchingcurrent statistics under equilibrium and nonequilibrium conditions. Our experimental data show ELQ in YBCO PSNs. The YBCO nanowires have a high crossover temperature between TA and quantum regimes of 12–13 K and their lifetime in the excited state exceeds 20 ms at 5.4 K, which is at least one orderofmagnitude longer than in lowT_{c} tunnel JJs^{1}. We also show that the absorption of a singlephoton changes the quantum and phaseslip states of YBCO nanowires. Our findings demonstrate that phaseslip YBCO nanowires are promising systems for quantum technology applications, including quantum sensing and computing.
Methods
Nanowire fabrication
YBCO nanowires were fabricated from an 8.2 nm (7 unit cell) thick YBCO film deposited on a TiO_{2}terminated (100) STO substrate by dc sputtering at high (3.4 mbar) oxygen pressure. YBCO deposition followed a procedure that is described elsewhere^{53}. A total of 100nmthick Au contact pads were deposited ex situ using room temperature dc magnetron sputtering with a shadow mask. Following contact pad deposition, nanowires were fabricated in a twostage process. In the first stage, 10μmwide 10μmlong microbridges integrated with a bowtie antenna and leads were patterned using optical UV contact lithography with a PMMA resist and Ar ion beam etching. In the second stage, 2μmlong nanowires aligned along STO crystallographic axes were fabricated across the microbridges with two cuts made with FIB milling using a Au/PMMA protective layer. A sketch of the device is shown in the Supplementary Fig. 5a. More details on the patterning process can be found in ref. ^{22}.
Experimental setups
We performed the measurements using two experimental setups. The first experimental setup was based on a liquid helium storage Dewar insert filled with He exchange gas, in which the nanowire and surrounding radiation shield had the same temperature. The second setup was based on an HLD5 liquid helium cryostat (Infrared Laboratories, Inc.). The sample was placed on a sample holder mounted on the 4 K stage of the cryostat and shielded by a radiation shield with a quartz window. The sample was illuminated through the window using continuous optical radiation emitted by LEDs and 77 K BBR from a 77 K radiation shield. The LEDs were placed in front of the window at a distance of 2 cm from the substrate and cooled to 77 K. The sample holder temperature was maintained to an accuracy of ±5 mK at 4.2 K and ±20 mK at 20 K for the Dewarinsertbased setup, and ±10 mK for the cryostatbased setup over the whole temperature range. The wiring inside the Dewar insert was made with twistedpair cables and had a bandwidth of 3.9 MHz. The nanowires inside the cryostat were connected to room temperature measuring equipment using highfrequency SMA coax cables and a 10 GHz probe. We used batteryoperated lownoise analog electronics with a 100 kHz frequency bandwidth to sweep the bias current and amplify the voltage across the nanowire. The rootmeansquare noise of the current source was 1 nA. The output signals of the analog electronics, proportional to the current and voltage across the nanowire, were digitized using a simultaneous 16bit data acquisition board DT9832 (Data Translation). All electrical connections, apart from the HF coax cables, were filtered using lowfrequency feedthrough filters. Cables between the analog electronics and cryogenic units were as short as possible to eliminate electromagnetic interference. The frequency spectrum of the output voltage signal was controlled before the measurement to ensure that no lowfrequency external noise was present in the measurement system.
Switchingcurrent measurement
In order to measure the switchingcurrent and retrappingcurrent statistics, the bias current through the nanowire was ramped linearly up and down over the range (0.85–1.05) I_{s} and IV curves were recorded with 2 × 10^{4} points per curve. The spacing between independent current points of 15.3 nA was determined by the 16bit resolution of the data acquisition board. The switching and retrapping currents were determined by postprocessing of the recorded data. Standard deviations of the retrapping current were computed in the standard way.
Nanowire capacitance calculation
The nanowire layout shown schematically in the Supplementary Fig. 5b is similar to that of a coplanar waveguide with ground. As a result of this similarity, we used a coplanar waveguide calculator^{54} to calculate the nanowire capacitance. The following parameters were used for the capacitance calculations: spacing S = 200 nm, substrate thickness H = 1 mm, and dielectric index of the STO substrate ε = 300. The spacing S consisted of the 60nmwide FIB cut and two 70nmwide damaged insulating regions of YBCO on the sides of the FIB cut^{22}. By using the coplanar waveguide calculator^{54}, we obtained a nanowire specific capacitance per unit length of C_{S} = 2.4 fF μm^{−1} and a total capacitance of the 2μmlong nanowire of C = 4.8 fF.
References
Devoret, M. H. & Schoelkopf, R. J. Superconducting circuits for quantum information: an outlook. Science 339, 1169–1174 (2013).
Likharev, K. K. Superconducting weak links. Rev. Mod. Phys. 51, 101–159 (1979).
Mooij, J. E. & Harmans, C. J. P. Phaseslip flux qubits. N. J. Phys. 7, 219 (2005).
Astafiev, O. V. et al. Coherent quantum phase slip. Nature 484, 355–358 (2012).
de Graaf, S. E. et al. Charge quantum interference device. Nat. Phys. 14, 590–595 (2018).
Ku, J., Manucharyan, V. & Bezryadin, A. Superconducting nanowires as nonlinear inductive elements for qubits. Phys. Rev. B 82, 134518 (2010).
Li, P. et al. Switching currents limited by single phase slips in onedimensional superconducting Al nanowires. Phys. Rev. Lett. 107, 137004 (2011).
Brenner, M. W., Roy, D., Shah, N. & Bezryadin, A. Dynamics of superconducting nanowires shunted with an external resistor. Phys. Rev. B 85, 224507 (2012).
Lin, S. Z. & Roy, D. Role of kinetic inductance in transport properties of shunted superconducting nanowires. J. Phys. Condens. Mat. 25, 325701 (2013).
Voss, R. F. & Webb, R. A. Macroscopic quantum tunneling in 1μm Nb JosephsonJunctions. Phys. Rev. Lett. 47, 265–268 (1981).
Martinis, J. M., Devoret, M. H. & Clarke, J. Energylevel quantization in the zerovoltage state of a currentbiased Josephson Junction. Phys. Rev. Lett. 55, 1543–1546 (1985).
Inomata, K. et al. Macroscopic quantum tunneling in a dwave HighT_{C} Bi_{2}Sr_{2}CaCu_{2}O_{8+δ} superconductor. Phys. Rev. Lett. 95, 107005 (2005).
Bauch, T. et al. Macroscopic quantum tunneling in dwave YBa_{2}Cu_{3}O_{7δ} Josephson junctions. Phys. Rev. Lett. 94, 087003 (2005).
Bauch, T. et al. Quantum dynamics of a dwave Josephson junction. Science 311, 57–60 (2006).
Kashiwaya, H. et al. Possible observation of energy level quantization in an intrinsic Josephson junction. Phys. C 468, 1919–1921 (2008).
Giordano, N. Superconducting fluctuations in onedimension. Phys. B 203, 460–466 (1994).
Aref, T., Levchenko, A., Vakaryuk, V. & Bezryadin, A. Quantitative analysis of quantum phase slips in superconducting Mo_{76}Ge_{24} nanowires revealed by switchingcurrent statistics. Phys. Rev. B 86, 024507 (2012).
Aref, T., Levchenko, A., Vakaryuk, V. & Bezryadin, A. Quantitative analysis of quantum phase slips in superconducting Mo_{76}Ge_{24} nanowires revealed by switchingcurrent statistics. Phys. Rev. B 86, 024507 (2012).
Tinkham, M. Introduction to superconductivity. (McGrawHill, Inc., 1996).
Deutscher, G. AndreevSaintJames reflections: a probe of cuprate superconductors. Rev. Mod. Phys. 77, 109–135 (2005).
Arpaia, R. et al. Ultra low noise YBa_{2}Cu_{3}O_{7δ} nano superconducting quantum interference devices implementing nanowires. Appl. Phys. Lett. 104, 072603 (2014).
Lyatti, M. et al. Experimental evidence for hotspot and phaseslip mechanisms of voltage switching in ultrathin YBa_{2}Cu_{3}O_{7x} nanowires. Phys. Rev. B 98, 054505 (2018).
Skocpol, W. J., Beasley, M. R. & Tinkham, M. Phaseslip centers and nonequilibrium processes in superconducting tin microbridges. J. Low. Temp. Phys. 16, 145–167 (1974).
Qiu, C. Y. & Qian, T. Z. Numerical study of the phase slip in twodimensional superconducting strips. Phys. Rev. B 77, 174517 (2008).
Weber, A. & Kramer, L. Dissipative states in a currentcarrying superconducting film. J. Low. Temp. Phys. 84, 289–299 (1991).
Andronov, A., Gordion, I., Kurin, V., Nefedov, I. & Shereshevsky, I. Kinematic vortices and phaseslip lines in the dynamics of the resistive state of narrow superconductive thinfilm channels. Phys. C 213, 193–199 (1993).
Ilichev, E. V., Kuznetsov, V. I. & Tulin, V. A. Conversion of phaseslip lines into elementary resistive domains in a currentcarrying superconducting thinfilm. JETP Lett. 56, 295–299 (1992).
Harshman, D. R. et al. Magnetic penetration depth in singlecrystal YBa_{2}Cu_{3}O_{7δ}. Phys. Rev. B 39, 851–854 (1989).
Ando, Y. & Segawa, K. Magnetoresistance of untwinned YBa_{2}Cu_{3}O_{y} single crystals in a wide range of doping: anomalous holedoping dependence of the coherence length. Phys. Rev. Lett. 88, 167005 (2002).
Kautz, R. L. & Martinis, J. M. Noiseaffected iv curves in small hysteretic JosephsonJunctions. Phys. Rev. B 42, 9903–9937 (1990).
Fulton, T. A. & Dunkleberger, L. N. Lifetime of zerovoltage state in Josephson tunneljunctions. Phys. Rev. B 9, 4760–4768 (1974).
Silvestrini, P., Palmieri, V. G., Ruggiero, B. & Russo, M. Observation of energy levels quantization in underdamped Josephson junctions above the classicalquantum regime crossover temperature. Phys. Rev. Lett. 79, 3046–3049 (1997).
Silvestrini, P., Ovchinnikov, Y. N. & Cristiano, R. Effects of level quantization on the supercurrent decay in josephsonjunctions  the nonstationary case. Phys. Rev. B 41, 7341–7344 (1990).
Martinis, J. M. & Kautz, R. L. Classical phase diffusion in small hysteretic Josephson junctions. Phys. Rev. Lett. 63, 1507–1510 (1989).
Yu, H. F. et al. Quantum phase diffusion in a small underdamped Josephson junction. Phys. Rev. Lett. 107, 067004 (2011).
Strauch, F. W. Theory Of Superconducting Phase Qubits (Univ. of Maryland, 2004).
Astafiev, O. et al. Single artificialatom lasing. Nature 449, 588–590 (2007).
Sun, G. Z. et al. Population inversion induced by LandauZener transition in a strongly driven rf superconducting quantum interference device. Appl Phys. Lett. 94, 102502 (2009).
Kozorezov, A. G. et al. Quasiparticlephonon downconversion in nonequilibrium superconductors. Phys. Rev. B 61, 11807–11819 (2000).
Kabanov, V. V. & Alexandrov, A. S. Electron relaxation in metals: theory and exact analytical solutions. Phys. Rev. B 78, 174514 (2008).
Semenov, A. D., Gol’tsman, G. N. & Korneev, A. A. Quantum detection by current carrying superconducting film. Phys. C 351, 349–356 (2001).
Semenov, A., Engel, A., Hubers, H. W., Il’in, K. & Siegel, M. Spectral cutoff in the efficiency of the resistive state formation caused by absorption of a singlephoton in currentcarrying superconducting nanostrips. Eur. Phys. J. B 47, 495–501 (2005).
Sobolewski, R. Quasiparticle thermalization and recombination in hightemperature superconductors excited by femtosecond optical pulses. Lect. Notes Phys. 545, 100–122 (2000).
Gedik, N., Orenstein, J., Liang, R. X., Bonn, D. A. & Hardy, W. N. Diffusion of nonequilibrium quasiparticles in a cuprate superconductor. Science 300, 1410–1412 (2003).
Semenov, A. D., Gol’tsman, G. N. & Sobolewski, R. Hotelectron effect in superconductors and its applications for radiation sensors. Supercond. Sci. Techn. 15, R1–R16 (2002).
Madan, I. et al. Nonequilibrium optical control of dynamical states in superconducting nanowire circuits. Sci. Adv. 4, eaao0043 (2018).
Tanner, D. B. et al. Superfluid and normal fluid density in highT_{c} superconductors. Phys. B 244, 1–8 (1998).
Gol’tsman, G. N. et al. Picosecond superconducting singlephoton optical detector. Appl. Phys. Lett. 79, 705–707 (2001).
Gay, P., Stevens, C. J., Smith, D. C., Chen, C. & Ryan, J. F. Anisotropy of nonequilibrium quasiparticle dynamics in singlecrystal YBa_{2}Cu_{3}O_{7δ}. Phys. C 341, 2269–2270 (2000).
Luo, C. W. et al. Spatial symmetry of the superconducting gap of YBa_{2}Cu_{3}O_{7δ} obtained from femtosecond spectroscopy. Phys. Rev. B 68, 220508(R) (2003).
Razzoli, E. et al. Evolution from a nodeless Gap to d_{x2}_{y2}wave in underdoped La_{2x}Sr_{x}CuO_{4}. Phys. Rev. Lett. 110, 047004 (2013).
Gustafsson, D. et al. Fully gapped superconductivity in a nanometresize YBa_{2}Cu_{3}O_{7δ} island enhanced by a magnetic field. Nat. Nanotechnol. 8, 25–30 (2013).
Lyatti, M., Savenko, A. & Poppe, U. Ultrathin YBa_{2}Cu_{3}O_{7x} films with high critical current density. Supercond. Sci. Techn. 29, 065017 (2016).
McMahill, D., Coplanar Waveguide Analysis/Synthesis Calculator, https://wcalc.sourceforge.net/cgi509bin/coplanar.cgi.
Acknowledgements
M.L. thanks G. Catelani for valuable discussions. This work was partially supported by ERC Project No. C088. C.S. acknowledges financial support from the Ministry for Innovation, Science and Research (North RhineWestphalia).We thank the Münster Nanofabrication Facility (MNF) for technical support during device fabrication.
Author information
Authors and Affiliations
Contributions
M.L. and M.K. fabricated the nanowires. M.L. and M.A.W. performed the measurements. S.F. and I.G. contributed to the experiments. M.L., I.G., R.E.D.B., and C.S. cowrote the paper. All authors commented on the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Peer review information Nature Communications thanks the anonymous reviewer(s) for their contribution to the peer review of this work. Peer reviewer reports are available.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Source data
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Lyatti, M., Wolff, M.A., Gundareva, I. et al. Energylevel quantization and singlephoton control of phase slips in YBa_{2}Cu_{3}O_{7–x} nanowires. Nat Commun 11, 763 (2020). https://doi.org/10.1038/s4146702014548x
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4146702014548x
Further reading

Roomtemperature oxygen vacancy migration induced reversible phase transformation during the anelastic deformation in CuO
Nature Communications (2021)

CurrentInduced Metastable States Close to T$$_{c}$$ in NbTi Superconducting Bridges
Journal of Superconductivity and Novel Magnetism (2021)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.